#------------------------------------------------------------------------------
#$Date: 2016-12-23 13:19:03 +0200 (Fri, 23 Dec 2016) $
#$Revision: 189357 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/54/48/1544852.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1544852
loop_
_publ_author_name
'Khobaer, T.M.'
'Kuribayashi, T.'
'Komatsu, K.'
'Kudoh, Y.'
_publ_section_title
;
 The partially dehydrated structure of natural heulandite: An in situ high
 temperature single crystal X-ray diffraction study Sample: room
 temperature
;
_journal_name_full
'Journal of Mineralogical and Petrological Sciences'
_journal_page_first              61
_journal_page_last               76
_journal_volume                  103
_journal_year                    2008
_chemical_formula_sum
'Al9.21 Ca3.64 H50.4 K0.4 Na1.14 O97.2 Si26.88 Sr0.21'
_chemical_name_common
(Na1.14K0.40Ca3.64Sr0.21)(Al9.21Si26.88)O72*25.2H2O
_chemical_name_mineral           'natural heulandite at RT'
_space_group_IT_number           12
_space_group_name_H-M_alt        'C 1 2/m 1'
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 116.43(1)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   17.716(4)
_cell_length_b                   17.780(3)
_cell_length_c                   7.438(2)
_cell_volume                     2098.0(8)
_cod_data_source_file            heulandite_RT.cif
_cod_data_source_block           heulandite_RT
_cod_original_formula_sum
'Na1.14 K0.40 Ca3.64 Sr0.21 Al9.21 Si26.88 O97.2 H50.4'
_cod_database_code               1544852
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'
'-x, y, -z'
'x, -y, z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, -z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_occupancy
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_type_symbol
T1 0.7450 0.17970(10) 0.16910(10) 0.0968(2) Uiso 0.012000 Si
T2 0.7450 0.21110(10) 0.40990(10) 0.4987(2) Uiso 0.012100 Si
T3 0.7450 0.20830(10) 0.19080(10) 0.7171(2) Uiso 0.011300 Si
T4 0.7450 0.06430(10) 0.29850(10) 0.4106(2) Uiso 0.011800 Si
T5 0.7450 0.000000 0.21190(10) 0.000000 Uiso 0.013000 Si
O1 1.0 0.1961(4) 0.500000 0.4498(9) Uiso 0.027500 O
O2 1.0 0.2305(2) 0.1197(4) 0.6115(7) Uiso 0.028600 O
O3 1.0 0.1841(4) 0.1535(4) 0.8839(7) Uiso 0.028500 O
O4 1.0 0.2397(2) 0.1060(4) 0.2561(7) Uiso 0.025500 O
O5 1.0 0.000000 0.3268(4) 0.500000 Uiso 0.029500 O
O6 1.0 0.0826(2) 0.1569(4) 0.0639(7) Uiso 0.023800 O
O7 1.0 0.1269(4) 0.2349(4) 0.5514(7) Uiso 0.035700 O
O8 1.0 0.0087(2) 0.2659(4) 0.1858(7) Uiso 0.030600 O
O9 1.0 0.2105(2) 0.2538(4) 0.1782(7) Uiso 0.025500 O
O10 1.0 0.1151(2) 0.3729(4) 0.3954(7) Uiso 0.026000 O
CaNa 0.4200 0.1540(2) 0.000000 0.6680(7) Uiso 0.054100 Ca
CaNa 0.2800 0.1540(2) 0.000000 0.6680(7) Uiso 0.054100 Na
CaNa 0.0520 0.1540(2) 0.000000 0.6680(7) Uiso 0.054100 Sr
Ca2 0.4800 0.0406(2) 0.500000 0.2010(7) Uiso 0.028900 Ca
K 0.1400 0.715(4) 0.000000 -0.059(7) Uiso 0.100000 K
W1 0.8400 0.2287(11) 0.500000 0.012(7) Uiso 0.040000 O
W2 0.8200 0.0817(8) 0.000000 0.873(3) Uiso 0.107000 O
W3 1.0 -0.0774(4) 0.5827(4) 0.0314(9) Uiso 0.058700 O
W4 1.0 0.000000 0.500000 0.500000 Uiso 0.080000 O
W5 0.1700 0.083(3) 0.042(3) 0.371(9) Uiso 0.090000 O
W6 0.8000 0.0995(9) 0.000000 0.286(3) Uiso 0.092000 O
W7 0.5000 0.0303(7) 0.0905(11) 0.505(3) Uiso 0.084000 O
